1 1 Basics of Corrosion Chemistry Norio Sato 1.1 Introduction Metallic materials in practical use are normally exposed to corrosion in the atmospheric and aqueous environments. Metallic corrosion is one of the problems we have often encountered in our industrialized society; hence it has been studied comprehensively since the industrial revolution in the late eighteenth century. Modern corrosion science was set off in the early twentieth century with the local cell model proposed by Evans  and the corrosion potential model proved by Wagner and Traud . The two models have joined into the modern electrochemical theory of corrosion, which describes metallic corrosion as a coupled electrochemical reaction consisting of anodic metal oxidation and cathodic oxidant reduction. The electrochemical theory is applicable not only to wet corrosion of metals at normal temperature but also to dry oxidation of metals at high temperature . Metallic materials corrode in a variety of gaseous and aqueous environments. In this chapter, we restrict ourselves to the most common corrosion of metals in aqueous solution and in wet air in the atmosphere. In general, metallic corrosion produces in its initial stage soluble metal ions in water, and then, the metal ions develop into solid corrosion precipitates such as metal oxide and hydroxide. We will discuss the whole process of metallic corrosion from the basic electrochemical standpoint. 1.2 Metallic Corrosion 1.2.1 Basic Processes The basic process of metallic corrosion in aqueous solution consists of the anodic dissolution of metals and the cathodic reduction of oxidants present in the solution: − MM → M2+ aq + 2eM anodic oxidation (1.1) Green Corrosion Chemistry and Engineering: Opportunities and Challenges, First Edition. Edited by Sanjay K. Sharma. 2012 Wiley-VCH Verlag GmbH & Co. KGaA. Published 2012 by Wiley-VCH Verlag GmbH & Co. KGaA. 2 1 Basics of Corrosion Chemistry − 2Oxaq + 2e− M → 2Red(eredox )aq cathodic oxidation (1.2) In the formulae, MM is the metal in the state of metallic bonding, M2+ aq is the is the electron in the metal, Ox hydrated metal ion in aqueous solution, e− aq is an M − ) is a reductant, and e is the redox electron in the reductant. oxidant, Red(e− aq redox redox The overall corrosion reaction is then written as follows: − MM + 2Oxaq → M2+ aq + 2Red(eredox )aq (1.3) These reactions are charge-transfer processes that occur across the interface between the metal and the aqueous solution, hence they are dependent on the interfacial potential that essentially corresponds to what is called the electrode potential of metals in electrochemistry terms. In physics terms, the electrode potential represents the energy level of electrons, called the Fermi level, in an electrode immersed in electrolyte. For normal metallic corrosion, in practice, the cathodic process is carried out by the reduction of hydrogen ions and/or the reduction of oxygen molecules in aqueous solution. These two cathodic reductions are electron transfer processes that occur across the metal–solution interface, whereas anodic metal dissolution is an ion transfer process across the interface. 1.2.2 Potential-pH Diagram Thermodynamics shows that an electrode reaction is reversible at its equilibrium potential, where no net reaction current is observed. We then learn that the anodic reaction of metallic corrosion may occur only in the potential range more positive than its equilibrium potential and that the cathodic reaction of oxidant reduction may occur only in the potential range more negative than its equilibrium potential. Moreover, it is known that metallic corrosion in aqueous solution is dependent not only on the electrode potential but also on the acidity and basicity of the solution, that is, the solution pH. The thermodynamic prediction of metallic corrosion was thus illustrated by Pourbaix  in the form of potential–pH diagrams, as shown for iron corrosion in Figure 1.1. The corrosion of metallic iron may occur in the potential–pH region where hydrated ferrous ions Fe2+ , ferric ions Fe3+ , and hydroxo-ferrous ions Fe(OH)− 3 are stable. No iron corrosion occurs in the region where metallic iron is thermodynamically stable at relatively negative electrode potentials. In the regions where solid iron oxides and hydroxides are stable, no iron corrosion into water is expected to develop and the iron surface is covered with solid oxide ﬁlms. In the diagram, we also see the equilibrium potentials of the hydrogen and oxygen electrode reactions. Atmospheric oxygen may cause iron corrosion in the potential range more negative than the oxygen equilibrium potential, EO2 /H2 O , while hydrogen ions in aqueous solution may carry iron corrosion in the potential range more negative than the hydrogen equilibrium potential, EH+ /H2 O . 1.2 Metallic Corrosion 2.0 1.6 Potential E / VNHE 1.2 Fe3+ EO2 /H2O 0.8 0.4 Fe2+ 0 Fe2O3 EH+/H2 −0.4 Fe O 3 4 −0.8 −1.2 Fe(OH)3− Fe −1.6 −2 0 2 4 6 8 10 12 14 16 pH Figure 1.1 Potential–pH diagram for iron corrosion in water at room temperature. EO2 /H2 O is the equilibrium potential for the oxygen electrode reaction, EH+ /H O is the 2 equilibrium potential for the hydrogen electrode reaction, and VNHE is volt on the normal hydrogen electrode scale . We note that the potential–pH diagram normally assumes metallic corrosion in pure water containing no foreign solutes. The presence of foreign solutes in aqueous solution may affect the corrosion and anticorrosion regions in the potential–pH diagram. We see in the literature a number of potential–pH diagrams for metallic corrosion in the presence of foreign solutes such as chloride and sulﬁdes [4, 5]. 1.2.3 Corrosion Potential An electrode of metal corroding in aqueous solution has an electrode potential, which is called the corrosion potential. As a matter of course, the corrosion potential stands somewhere in the range between the equilibrium potential of the anodic metal dissolution and that of the cathodic oxidant reduction. It comes from the kinetics of metallic corrosion that at the corrosion potential, the anodic oxidation current of the metal dissolution is equal to the cathodic reduction current of the oxidant. The corrosion kinetics is usually described by the electrode potential versus reaction current curves of both the anodic oxidation and the cathodic reduction, as schematically shown in Figure 1.2, which electrochemists call the polarization curves of corrosion reactions. We see in Figure 1.2 that the intersecting point of the anodic and cathodic polarization curves represents the state of corrosion, namely, the corrosion potential and the corrosion current. We then realize that the corrosion 3 1 Basics of Corrosion Chemistry Ec Potential E 4 ic Ecorr ia Ea icorr i Figure 1.2 Conceptual potential–current curves of anodic and cathodic reactions for metallic corrosion; ia is the anodic reaction current, ic is the cathodic reaction current, icorr is the corrosion current, Ea is the equilibrium potential of the anodic reaction, Ec is the equilibrium potential of the cathodic reaction, and Ecorr is the corrosion potential. potential is determined by both the anodic and cathodic polarization curves of the corrosion reactions. The corrosion rate of metals may be controlled by either the anodic or the cathodic reaction. In most cases of metallic corrosion, the cathodic hydrogen ion reduction controls the rate of metallic corrosion in acidic solution, while in neutral solution, the cathodic oxygen reduction preferentially controls the corrosion rate. If the corrosion potential comes out far away from the equilibrium potential of the cathodic reaction, the corrosion rate will be controlled by the cathodic reaction. In practice, we see that metallic corrosion is often controlled by the oxygen diffusion toward the corroding metal surface, in which the corrosion potential is far more negative than the oxygen equilibrium potential. 1.2.4 Anodic Metal Dissolution Electrochemical kinetics gives the reaction current, ia , of anodic metal dissolution as an exponential function of the electrode potential, E, of the metal as follows: αa E (1.4) ia = Ka exp kT In Eq. (1.4), Ka and αa are parameters. The anodic dissolution current of metallic iron, in fact, increases exponentially with the anodic electrode potential in acid solution as shown in Figure 1.3 . Anodic metal dissolution depends not only on the electrode potential but also on the acidity and foreign solutes present in the aqueous solution. It is a received 1.2 Metallic Corrosion Potential E / V SCE −0.1 −0.2 ia −0.3 Ecorr −0.4 ic icorr −0.5 −0.6 Fe / H2SO4 0 1 2 log |i / 10−2 3 A 4 cm−2| Figure 1.3 Potential–current curves for corroding iron in sulfuric acid solution at pH 1.7 at 25 ◦ C; VSCE is the volt on the saturated calomel electrode scale . understanding that the anodic dissolution current of metallic iron depends on the concentration of hydroxide ions in the solution. Hydrated anions other than hydroxide ions also have some effects on the anodic metal dissolution. Hydrated hydroxide ions are found to accelerate the anodic iron dissolution in weekly acidic solution; whereas they decelerate (hydrated hydrogen ions accelerate) the iron dissolution in strongly acidic solution . Furthermore, in acidic solution, hydrated chloride ions accelerate the anodic iron dissolution in relatively concentrated chloride solution, while they inhibit the iron dissolution in relatively dilute chloride solution . These facts suggest that anions of different sorts compete with one another in participating in the process of anodic metal dissolution probably through their adsorption on the metal surface forming activated inter+ mediates, such as FeOH+ ad and FeClad , which will determine the metal dissolution rate . It is worth noting that, in general, the surface of metal is soft acid in the Lewis acid–base concept  and tends to adsorb ions and molecules of soft base, forming covalent bonds between the metal surface and the adsorbates. It is also noteworthy that as the anodic metal potential increases in the more positive direction, the Lewis acidity of the metal surface may gradually turn from soft acid to hard acid. The anions of soft base adsorbed in the range of less positive potentials are then replaced in the range of more positive potentials by anions of hard base such as hydroxide ions and water molecules. In general, iodide ions I− , sulﬁde ions S− , and thiocyanate ions SCN− are the soft bases, while hydroxide ions OH− , ﬂuoride 2− ions F− , chloride ions Cl− , phosphate ions PO3− 4 , sulfate ions SO4 , and chromate 5 6 1 Basics of Corrosion Chemistry 2− − ions CrO2− 4 are the hard bases. Bromide ions Br and sulfurous ions SO3 stand somewhere between the soft base and the hard base. 1.2.5 Cathodic Oxidant Reduction The cathodic current, ic , of oxidant reduction is also an exponential function of the electrode potential, E, of the metal as follows: −αc E (1.5) ic = Kc exp kT For metallic iron in acid solution, where the hydrogen ion reduction carries the cathodic reaction of corrosion, the cathodic current increases exponentially with increasing cathodic electrode potential in the more negative direction as shown in Figure 1.3. The cathodic reaction for usual metallic corrosion is carried by the hydrogen reaction and/or the oxygen reaction. For the hydrogen reaction, there are two cathodic processes that produce hydrogen gas at metal electrodes: one is the reduction of hydrogen ions and the other is the reduction of water molecules. − 2H+ aq + 2eM → H2,gas 2H2 O + 2e− M (1.6) → H2,gas + 2OH− aq (1.7) Hydrogen ion reduction preferentially occurs in acidic solution, and its reaction current increases with increasing hydrogen ion concentration. Water molecule reduction occurs in weakly acidic and neutral solutions. The cathodic polarization curves (potential–current curves) of these two reactions are different from each other. The cathodic current of hydrogen ion reduction increases with increasing cathodic electrode potential until it reaches a limiting current of hydrogen ion diffusion toward the metal surface, and beyond a certain cathodic potential, the cathodic current of water molecule reduction emerges and increases with the cathodic electrode potential . For oxygen reduction, similarly, there are two cathodic processes: one involves hydrogen ions and the other requires water molecules. − O2,gas + 4H+ aq + 4eM → 2H2 O O2,gas + 2H2 O + 4e− M → 4OH− aq (1.8) (1.9) The oxygen reduction involving hydrogen ions takes place preferentially in acidic solution with the reaction current limited not only by the oxygen diffusion but also by the hydrogen ion diffusion toward the metal surface; whereas the oxygen reduction requiring water molecules develops in neutral and alkaline solutions and its reaction current is limited by the oxygen diffusion . It is most likely in practical environments that the corrosion of metals is controlled by the diffusion of oxygen toward the surface of corroding metals. 1.3 Metallic Passivity 1.3 Metallic Passivity 1.3.1 Passivity of Metals Metallic passivity was discovered in 1790 by Keir , who found that metallic iron violently corroding in the active state in concentrated nitric acid solution suddenly turned into the passive state where almost no corrosion was observed. It was not until 1960s that we conﬁrmed the presence of an oxide ﬁlm several nanometers thick on the surface of passivated metals . Latest overviews on metallic passivity may be referred to in the literature of corrosion science . We illustrate metallic passivity with the potential–current curve of anodic metal dissolution for metallic iron, nickel, and chromium in acid solution as shown in Figure 1.4. Anodic metal passivation occurs at a certain potential, called the passivation potential, EP , beyond which the anodic current of metal dissolution drastically decreases to a negligible level. It is an observed fact that the passivation potential depends on the solution acidity, lineally shifting in the more positive direction with decreasing solution pH. This fact thermodynamically suggests that metallic passivity is caused by the formation of an oxide ﬁlm on the metal, which is extremely thin and invisible to the naked eye. +2.5 Fe, Ni, Cr / 0.5 kmol m−3 +2.0 H2SO4, 25 °C Potential E / VSCE O2 +1.5 +1.0 +0.5 Cr Fe Ni 0 −0.5 −8 −6 −4 −2 0 log |ia / 10−2 A cm−2| Figure 1.4 Potential–current curves for anodic dissolution of iron Fe, nickel Ni, and chromium Cr in 0.5 mol m−3 sulfuric acid solution at 25 ◦ C; O2 is anodic oxygen evolution current. 7 8 1 Basics of Corrosion Chemistry In the potential range of passivity, a nanometer-thin oxide ﬁlm is formed on the metal, which is called the passive ﬁlm. The ﬁlm grows in thickness with increasing anodic potential at the rate of 1–3 nm V−1 equivalent to an electric ﬁeld of 106 –107 V cm−1 across the ﬁlm . For most of the iron group metals, the passive ﬁlm is less than several nanometers in thickness in the potential region where it is stable. For some metals such as aluminum and titanium, the passive oxide ﬁlm can be made thick up to several hundred nanometers by increasing anodic potential; the thick oxide is frequently called the anodic oxide. In the potential range where the passive state is stable, as shown in Figure 1.4, the metal anode normally holds an extremely small, potential-independent metal dissolution current, which is equivalent to the dissolution rate of the passive ﬁlm itself. We see that the anodic metal dissolution current in the passive state is controlled by the dissolution rate of the passive ﬁlm. The potential-independent dissolution of passive metals results from the fact that the interfacial potential between the passive oxide ﬁlm and the solution, which controls the ﬁlm dissolution rate, remains constant independent of the anodic potential, although depending on the solution pH [12, 14, 15]. For some metals, the passive state turns beyond a certain potential to be what is called the transpassive state, where the anodic dissolution current for the most part increases exponentially with the anodic potential as shown in Figure 1.4. The anodic metal dissolution in the transpassive state is thus controlled by the potential-dependent dissolution of the transpassive ﬁlm. In the transpassive potential range, the interfacial potential between the ﬁlm and the solution is not constant but depends on the anodic potential of the metal. The passive ﬁlm is stable as long as the Fermi level (the electrode potential) of the metal anode is within the band gap of electron energy between the conduction and valence bands of the ﬁlm, a situation which realizes the nonmetallic nature of the interface and hence makes the interfacial potential independent of the metal potential [12, 14, 15]. As the anodic potential increases, the Fermi level ﬁnally reaches the valence band edge of the ﬁlm at the ﬁlm–solution interface and the quasi-metallization (electronic degeneracy) is realized at the same. The ﬁlm–solution interfacial potential, hence, turns to be dependent on the anodic metal potential, and as a result, potential-dependent transpassive dissolution occurs beyond the transpassivation potential, ETP . Let us see the anodic metal dissolution of iron, nickel, and chromium in acid solution as shown in Figure 1.4. While going into solution as hydrated ferrous ions in the active state, metallic iron in the passive state dissolves in the form of hydrated ferric ions, indicating that the passive ﬁlm is ferric oxide, Fe2 O3 . − 2Fe + 3H2 O → Fe2 O3 + 6H+ aq + 6eM Fe2 O3 + 6H+ aq → 2Fe3+ aq + 3H2 O passive ﬁlm formation passive ﬁlm dissolution (1.10) (1.11) These two reactions proceed simultaneously, maintaining the passive ﬁlm at a steady thickness, which increases with increasing anodic potential. 1.3 Metallic Passivity Anodic nickel dissolution produces divalent nickel ions both in the active and passive states, implying that the passive ﬁlm is divalent nickel oxide. − Ni + H2 O → NiO + 2H+ aq + eM NiO + 2H+ aq → Ni2+ aq passive ﬁlm formation + H2 O passive ﬁlm dissolution (1.12) (1.13) In the transpassive state, as mentioned earlier, the ﬁlm dissolution rate is potential dependent in contrast to the passive state in which it is potential independent. Since the dissolution current increases with the anodic potential, the thickness of the transpassive ﬁlm seems to decrease with the anodic potential in the steady state. Beyond the transpassive potential range of nickel, the transpassive divalent oxide ﬁlm is assumed to change near the oxygen evolution potential into a trivalent oxide ﬁlm causing a decrease in the anodic nickel dissolution current . For chromium, the anodic dissolution produces divalent chromium ions in the active state and the passivation occurs forming an extremely thin, trivalent chromium oxide ﬁlm on the metal surface. − 2Cr + 3H2 O → Cr2 O3 + 6H+ aq + 6eM passive ﬁlm formation 3+ Cr2 O3 + 6H+ aq → 2Craq + 3H2 O passive ﬁlm dissolution Cr2 O3 + 5H2 O + 6e− M → 2CrO4,aq 2− + 10H+ aq (1.14) (1.15) transpassive ﬁlm dissolution (1.16) The transpassive dissolution of metallic chromium is the oxidative dissolution of trivalent chromic oxide into soluble hexavalent chromate ions in acidic solution; hence the anodic transpassive dissolution proceeds through the formation of a chromic oxide ﬁlm on the metal surface. 1.3.2 Passivation of Metals A metallic electrode may be made passive if its corrosion potential is held in the potential range of passivity. The corrosion potential is determined, as mentioned earlier, by both the anodic metal dissolution current and the cathodic oxidant reduction current. As shown in Figure 1.5, the corrosion potential remains in the active state as long as the cathodic current is less than the maximum current of anodic metal dissolution; whereas it goes to the passive potential range when the cathodic current exceeds the anodic dissolution current. An unstable passive state arises if the cathodic potential–current curve crosses the anodic potential–current curve at two potentials, one in the passive state and the other in the active state. A metallic electrode in the unstable passive state, once its passivity breaks down, never repassivates because the cathodic current of oxidant reduction is insufﬁcient in magnitude for the activated metal to clear its anodic dissolution current peak. It has been observed that metallic nickel corrodes in acidic solution but passivates in basic solution: the transition from the active corrosion to passivation occurs at pH 6 in sulfate solution . The corrosion of nickel in weakly acidic and neutral solutions is controlled by cathodic oxygen reduction whose current is limited by 9 1 Basics of Corrosion Chemistry ic ic Potential E 10 ia ia ic ia log i (a) log i (c) log i (b) Figure 1.5 Passivation of metals and its stability. (a) Active corrosion, (b) unstable passivity, (c) stable passivity; ia is the anodic current and ic is the cathodic current. the oxygen diffusion toward the metal surface. The nickel dissolution current peak in the active state decreases with increasing solution pH and becomes less than the cathodic oxygen diffusion current beyond pH 6. Consequently, metallic nickel passivates in a solution more basic than pH 6, which is called the passivation pH of nickel. Let us see the oxidizing agent of nitrite ion NO− 2 that provides a cathodic reaction for the corrosion and passivation of metallic iron in weakly acidic and neutral solutions. − − NO− 2,aq + 5H2 O + 6eM → NH3 + 7OHaq 2Fe → 2Fe2+ aq + cathodic reaction (1.17) 4e− M − 2Fe + 3H2 O → Fe2 O3 + 6H+ aq + 6eM anodic reaction (1.18) Metallic iron remains in the active state if the cathodic reaction current is insufﬁcient for the metal to passivate; whereas it turns out to be passive forming a surface ﬁlm of ferric oxide if the cathodic reaction current surmounts the metal dissolution current peak. Owing to its relatively more-positive redox potential and its greater reaction current, an amount of nitrite salt readily brings metallic iron into the passive state, and thus, it provides an effective passivating reagent for iron and steel. It is also noted that chromate ions, CrO2− 4 , oxidize metallic iron to form a passive ﬁlm of chromic–ferric mixed oxides on the metal surface. CrO4,aq 2− + 10H2 O + 6e− M → Cr2 O3 + 5H2 O 2Fe + 3H2 O → Fe2 O3 + 6H+ aq + 6e− M cathodic reaction anodic reaction (1.19) (1.20) Chromate is one of the strongest oxidants to passivate metallic materials. In the same way, molybdate and tungstate may also make metallic iron passive, although their oxidizing capacity may not always be sufﬁcient. 1.3 Metallic Passivity 1.3.3 Passive Films The passive oxide ﬁlm on metals is very thin, of the order of several nanometers, and hence, sensitive to the environment in which it is formed. In the formation and growth processes of the ﬁlm, the oxide ions migrate from the solution across the ﬁlm to the metal–oxide interface forming an inner oxide layer, while the metal ions migrate from the metal to the oxide–solution interface to react with adsorbed water molecules and solute anions forming an outer oxide layer, which occasionally incorporates anions other than oxide ions into itself. The anion incorporation occurs only when the migrating metal ions react with the adsorbed anions. The ratio of the thickness of the outer anion-incorporating layer to the overall layer is expressed by the transport number, τM , of the metal ion migration during the ﬁlm growth. The transport number was found to be τM = 0.7–0.8 for an anodic oxide ﬁlm 65 nm thick formed on aluminum in phosphate solution . The passive ﬁlm is mostly amorphous, but as the ﬁlm grows thicker, it may turn to be crystalline. For the passivity of metallic titanium in sulfuric acid solution, the passive ﬁlm appears to change from amorphous to crystalline beyond the anodic potential of about 8 V, probably because of the internal stress created in the ﬁlm . The passive ﬁlm is either an insulator or a semiconductor. For metallic iron, titanium, tin, niobium, and tungsten, the passive ﬁlm is an n-type semiconductor with donors in high concentration. Some metals such as metallic nickel, chromium, and copper make the passive ﬁlm a p-type semiconductor oxide. The passive ﬁlms on metallic aluminum, tantalum, and hafnium are insulator oxides. We may classify the passive oxide ﬁlms into two categories: the network former (glass former) and the the network modiﬁer . The network former, which includes metallic silicon, aluminum, titanium, zirconium, and molybdenum, normally forms a single-layered oxide ﬁlm. On the other hand, the network modiﬁer, which includes metallic iron, nickel, cobalt, and copper, tends to form a multilayered oxide ﬁlm, such as a cobalt oxide ﬁlm, consisting of an inner divalent oxide layer and an outer trivalent oxide layer (Co/CoO/Co2 O3 ). High-valence metal oxides normally appear to be more corrosion resistive than low-valence metal oxides. The anodic formation of network-forming oxides is most likely carried through the inward oxide ion migration to the metal–oxide interface and hence will probably produce a dehydrated compact ﬁlm containing no foreign anions other than oxide ions; whereas, network-modifying oxides appear to grow through the outward metal ion migration to the oxide–solution interface forming a more or less defective ﬁlm occasionally containing foreign anions. It is worth noting that since the passive ﬁlm is so extremely thin, electrons easily transfer across the ﬁlm by the quantum mechanical electron tunneling mechanism, irrespective of whether the passive ﬁlm is an insulator or a semiconductor. By contrast, however, no ionic tunneling is allowed to occur across the passive ﬁlm. The passive ﬁlm thus constitutes a barrier layer to ion transfer but not to electron transfer. Any redox electron transfer reaction is therefore allowed to occur on the passive ﬁlm-covered metal surface just like on the metal surface without any ﬁlm. 11 1 Basics of Corrosion Chemistry 1.3.4 Chloride-Breakdown of Passive Films The passive ﬁlm on metals may break down in the presence of aggressive ions, such as chloride ions, in solution, and the breakdown site may trigger a localized corrosion of the underlying metals. The chloride-breakdown of passive ﬁlms, in general, occurs beyond a certain potential, which we call the ﬁlm breakdown potential, Eb . Either repassivation or pitting corrosion then follows at the breakdown site, as schematically shown in Figure 1.6. Pitting corrosion is also characterized by a threshold potential, called the pitting potential, Epit , above which pitting grows but below which pitting ceases to occur. These two potentials, Eb and Epit , are inﬂuenced by the concentrations of chloride ions and hydrogen ions in the solution. There is a marginal chloride concentration below which no ﬁlm breakdown occurs. For chloride-breakdown of the passive ﬁlm on metallic iron, the concentration of chloride ions required for the ﬁlm breakdown depends on the ﬁlm thickness, defects in the ﬁlm, the electric ﬁeld intensity in the ﬁlm, and pH of the solution . It is also found that the passive ﬁlm locally dissolves and thins down before the underlying metal begins pitting at the ﬁlm breakdown site [21, 22]. It is then likely that the ﬁlm breakdown results not from a mechanical rupture but from a localized mode of ﬁlm dissolution because of the adsorption of chloride ions. It is frequently seen that the passive ﬁlm preferentially breaks down at the sites of crystal grain boundaries, nonmetallic inclusions, and ﬂaws on the metal surface. For stainless steels, the passivity breakdown and pit initiation most likely occur at the site of nonmetallic inclusions of MnS. It is noted that any localized phenomena are nondeterministic and in general, somehow stochastic. Chloride-breakdown of passive ﬁlms on stainless steels was found to come out in accordance with a stochastic distribution [23, 24]. The pitting potential, Epit , at which pitting begins to grow, arises at a potential either more positive (more anodic) or less positive (more cathodic) than the ﬁlm Transpassive state ETP Pitting corrosion Epit Potential E 12 Unstable pitting Eb Stable passive state EP Active state log i Figure 1.6 Schematic potential–current curves for metallic passivation, passive-ﬁlm breakdown, pitting dissolution, and transpassivation; Eb is the ﬁlm breakdown potential, Epit is the pitting potential, EP is the passivation potential, and ETP is the transpassivation potential. 1.4 Localized Corrosion breakdown potential, Eb . When the ﬁlm breakdown potential is less-positive than the pitting potential, the breakdown site repassivates, as we observe for some stainless steels in acid solution . On the other hand, pitting corrosion follows ﬁlm breakdown when the ﬁlm breakdown potential emerges more positive than the pitting potential, as we observe for metallic iron in acid solution . For the mechanism of chloride-breakdown of passive ﬁlms, one of the currently prevailing models is the ionic point defect model that assumes injection of metal ion vacancies into the passive ﬁlm at the adsorption site of chloride ions. The ionic point defects thus injected migrate to and accumulate at the metal–ﬁlm interface, ﬁnally creating a void there to break the ﬁlm down . Another model is the electronic point defect model that assumes injection of an electronic defect level localized at the ﬁlm–solution interface. The electronic interfacial state thus injected causes local quasi-metallization at the adsorption site of chloride ions, ﬁnally resulting in a local mode of ﬁlm dissolution [14, 15, 27]. There have also been several chemical models for passivity breakdown, which more or less assume the formation of a soluble chloride complex at the chloride adsorption site. We note at the end that the passivity breakdown is different from the pitting that follows: the former is a process associated with the passive ﬁlm itself, whereas the underlying metal is responsible for the latter. 1.4 Localized Corrosion 1.4.1 Pitting Corrosion Pitting corrosion of metals in general occurs in the potential range more positive than the pitting potential, Epit . For usual stainless steel in 1 mol dm−3 sodium chloride solution, the pitting potential arises around +0.3 V on the normal hydrogen electrode (NHE) scale . Once metallic pitting sets in, the anodic metal dissolution current increases with the anodic potential as schematically shown in Figure 1.6. The pit initially grows in a semispherical shape with the pit solution that acidiﬁes and concentrates in soluble metal salts. For 304 stainless steels in neutral chloride media at pH = 6 ∼ 8, the local pH in the pit falls down to pH = 1 ∼ 2 . The kinetics of pit dissolution appears to be different from that of metal dissolution in the active state. The pitting dissolution current density, ipit , is given by an exponential function of the anodic potential, E. E = a + b log ipit (1.21) In acid solution, the coefﬁcient b (Tafel constant) is 0.20 V for metallic iron  and 0.30 V for stainless steel . These Tafel constants are much greater than those (0.03 ∼ 0.1 V) normally observed for anodic metal dissolution in the active state. The metal dissolution in the pit proceeds in an acidiﬁed, concentrated salt 13 1 Basics of Corrosion Chemistry Epit Potential E 14 (rpit) ER ′) (rpit ER′ Pitting Passive state E P* EP Active state log I Figure 1.7 Schematic potential–current curves for metallic pitting dissolution, and pit > rpit ), EP∗ is the passivation–depassivation potential repassivation; rpit is the pit radius (rpit for the critical pit solution, and EP is the passivation–depassivation potential for the solution outside the pit. solution with an electropolishing mode of dissolution, which is different from the usual mode of metal dissolution in the potential range of the active state. As the electrode potential of pitting metal is made more negative, we come to a certain potential at which the pitting metal dissolution ceases to occur, resulting in repassivation of the pit, a certain potential which we call the pit-repassivation potential, ER . The pit-repassivation potential is found to move more negative with increasing pit size, as schematically shown in Figure 1.7. We may then assume that a pit embryo takes a certain critical size at the pitting potential, Epit , at which the pitting starts to occur. For stainless steel in acidic chloride solution, the smallest pit size for the initiation of pitting was estimated at 0.01–0.02 mm . From the kinetics of pitting dissolution and mass transport in a semispherical pit, it is deduced that the pit-repassivation potential ER is a logarithmic function of pit radius rpit . ER = a + b log rpit (1.22) We in fact observe that a logarithmic dependence of the pit-repassivation potential on the pit radius is held for stainless steel in acid solution . It appears that the pitting mode of metal dissolution requires highly concentrated acidic chloride in the pit solution, whose chloride ions must be more concentrated ∗ than a certain critical value, cCl − . For usual stainless steel in acid solution, the −3 ∗ critical chloride concentration was estimated to be cCl . − = 1.8 kmol m The pit solution is also highly acidiﬁed to keep running a polishing mode of pitting dissolution and preventing the pit from repassivation at potentials more ∗ positive than ER . The critical chloride concentration, cCl − , is thus accompanied 1.4 Localized Corrosion ∗ with a critical level of acidity, cH + , above which no pit repassivation occurs. The ∗ ∗ critical chloride–hydrogen ion concentration, cH + (cCl− ), will then determine the ∗ ∗ pit stability. Pitting corrosion continues occurring if cH+ (cCl− ) ≥ cH + (cCl− ), but ∗ ∗ (c ). repassivation occurs if cH+ (cCl− ) < cH + Cl− Metallic passivity in general occurs beyond the passivation potential, EP , which becomes more positive with increasing solution acidity as mentioned earlier. It may hence be accepted that even for the critically acidiﬁed pit solution, the passivation potential may occur, which we call the critical passivation–depassivation potential, EP∗ , for the acidiﬁed pit solution. The EP∗ obviously stands much more positive than the normal passivation potential, EP , for the solution outside the pit. It appears, then, that as the repassivation potential, ER , of the pit goes down more negative than the critical depassivation potential EP∗ , pit repassivation never occurs, and that pitting corrosion in the electropolishing mode turns to be the usual mode of active metal dissolution with the metal potential falling down into the range of the active state. Figure 1.8 schematically shows that the pit-repassivation potential ER intersects ∗ , which is the with the critical depassivation potential EP∗ at a certain pit radius, rpit largest size of the pit that is repassivable. A corroding pit never repassivates if it ∗ . grows greater than its largest repassivable size rpit The foregoing discussion indicates that both the pit-repassivation potential ER and the critical depassivation potential EP∗ play a primary role in the stability of pitting corrosion of metals. For pitting corrosion to occur, a pit embryo ﬁrst breaks out at a potential in the range of passivity, where the metal surface remains passive except for the pit site. As the pit grows in size, its repassivation r 0pit Epit Ecorr Pitting ER Potential E E ′corr r*pit Repassivation E *P EP Active state log rpit ∗ is Figure 1.8 Schematic potential–size curves for metallic pitting and pit repassivation: rpit 0 the maximum radius of repassivable pits, rpit is the critical size of pit embryos, and Ecorr is the corrosion potential of pitting metal. 15 16 1 Basics of Corrosion Chemistry potential ER goes down more negative, while the critical depassivation potential EP∗ stays constant for the occluded pit solution at the critical chloride–hydrogen ion ∗ ∗ concentration, cH + (cCl− ). It then appears that a corroding pit repassivates in the potential range between ER and EP∗ as long as its repassivation potential is more positive than the critical depassivation potential (ER > EP∗ ). By contrast, a corroding pit never passivates if its repassivation potential goes down more negative than the critical depassivation potential (ER < EP∗ ), and consequently, no pit repassivation is expected to occur for the corrosion pit growing greater than the largest repassivable ∗ . The mode of local corrosion then changes from pitting corrosion to active size, rpit pit corrosion, namely, from electropolishing to active dissolution. The corrosion potential, as mentioned earlier, is controlled by the cathodic oxidant reduction. In the case of pitting corrosion, the cathodic reaction mainly occurs on the passive metal surface other than the pitting site. It is also known that the corrosion potential is made more positive and stable with increasing intensity and capacity of the oxidant reduction that supplies the cathodic current for corrosion. With the greater capacity of the cathodic reaction, the corrosion potential remains stable at relatively more positive potentials and the pit may be allowed to grow until its size exceeds the limiting value of repassivable pits, ∗ , before the potential falls down to its repassivation potential. Hence, no pit rpit repassivation occurs as schematically shown in Figure 1.8. With the smaller capacity of the cathodic reaction, in contrast, the corrosion potential falls more steeply to ∗ , and the pit-repassivation potential before the pit grows over its limiting size of rpit hence pit repassivation results. We also note that the pitting potential is made more positive by lowering temperature until it reaches a certain temperature, called the critical pitting temperature, below which no pitting occurs . For 316 stainless steels in sea water, the critical pitting temperature was about 30 ◦ C . Criterions of the temperature and potential for pitting corrosion all result from the stability requirement of pitting as described above. 1.4.2 Crevice Corrosion Crevice corrosion is a type of localized corrosion that arises in structural crevices in the presence of chloride ions in aqueous solution. It normally occurs when the gap of a crevice is thinner than a certain width of the order of micrometers, which was estimated at 30–40 µm for usual stainless steel in acid solution . The anodic metal dissolution in a crevice is usually coupled with the cathodic oxidant reduction that occurs outside the crevice, forming a local corrosion cell that involves the migration of hydrated ions through the crevice. For crevice corrosion to occur, a certain induction period is hence required to create a local corrosion cell between the inside and the outside of the crevice. In general, crevice corrosion ceases growing in the potential range more negative than a certain critical potential, which we call the crevice protection potential, Ecrev . Figure 1.9 schematically shows that the crevice is protected from corroding as the 1.4 Localized Corrosion Crevice in stainless steel 1Ecrev − 1CCl Potential E * 1I crev 2Ecrev − 2CCl * 2I crev 3Ecrev − 3CCl * 3I crev 3CCl− > 2CCl− > 1CCl− log I crev Figure 1.9 Schematic potential–current curves for anodic dissolution of a cylindrical crevice in stainless steel in neutral solutions at three different chloride ion concentrations; Icrev is the anodic crevice corrosion current, cCl− is the chloride ion concentration outside the crevice, Ecrev is the crevice protection potential, and I∗crev is the crevice corrosion current at Ecrev . potential of the corroding crevice is made more negative than the crevice protection potential. The protection potential, Ecrev , goes more negative with increasing chloride ion concentration, cCl− outside the crevice . 0 Ecrev = Ecrev − α log cCl− (1.23) ∗ , at the protection potential Ecrev is The threshold crevice corrosion current, Icrev also found to be a linear function of the chloride ion concentration . ∗ 0 Icrev = Icrev − βcCl− 1 β∝ hcrev (1.24) The coefﬁcient, β, is found to be inversely proportional to the crevice depth, hcrev . It is the acidiﬁcation of the occluded crevice solution that sets off crevice corrosion. The critical acidity that sets off crevice corrosion is equal to what is called the passivation–depassivation pH, above which the crevice passivates spontaneously and below which it remains in the active state. The passivation potential of the crevice metal at the passivation–depassivation pH provides the characteristic ∗ , within the crevice. The actual potential that we measure protection potential, Ecrev involves an IR drop, EIR , caused by the ionic current through the crevice. From the kinetics of metal dissolution and mass transport, it is revealed that the crevice protection potential, Ecrev , for a cylindrical crevice is a logarithmic function of the crevice depth, hcrev [35, 36]. ∗ Ecrev = Ecrev + EIR = a − b log hcrev (1.25) 17 1 Basics of Corrosion Chemistry We see that a linear relationship holds between the crevice protection potential, Ecrev , and the logarithm of the crevice depth, log hcrev , for a corrosion crevice of stainless steel in acid solution [35, 36]. No crevice corrosion occurs below a certain temperature called the critical crevice corrosion temperature, a situation which equates with the critical pitting temperature described earlier. The critical crevice temperature for stainless steel in seawater appears to be lower than the critical pitting temperature . The crevice corrosion temperature has actually been used as a measure to evaluate metallic materials for their susceptibility to crevice corrosion. 1.4.3 Potential–Dimension Diagram From the foregoing discussion, we illustrate the stability of pitting and crevice corrosion in a potential–dimension diagram made up of the corrosion potential and the dimension of pitting and crevice corrosion, as schematically shown in Figure 1.10 [35, 36]. In general, as mentioned earlier, a corrosion pit ﬁrst breaks out on the passivated surface of metals at the corrosion potential more positive than the pitting potential, Epit , and it then grows in its size with a fall of the corrosion potential in the more negative direction. If the supply of the cathodic current is insufﬁcient for corrosion, the corrosion potential is rather unstable and readily falls down in the more negative direction with a relatively small rate of pit growth. Since the repassivation potential, ER , of the small pit stands more positive than the critical depassivation potential EP∗ for the pit solution, the falling corrosion potential reaches ER before arriving at EP∗ , and consequently, the small pit repassivates into the noncorrosive state. In contrast, if a sufﬁcient supply of the cathodic current is available for pitting corrosion, the pit grows rather fast at relatively positive potentials until its size Epit Pitting Potential E 18 ER r *pit Pit repassivation E *P Crevice corrosion Pitting No crevice corrosion Ecrev log rpit, log hcrev Figure 1.10 Schematic potential–dimension diagram for localized corrosion of stainless steel in aqueous solution [35, 36]. 1.5 Corrosion Rust ∗ exceeds the critical value, rpit , beyond which no pit repassivation is expected to occur. The corrosion potential then gradually falls down to the critical depassivation potential, EP∗ , before reaching the pit-repassivation potential, ER , and hence the pitting corrosion ﬁnally changes to the active mode of pit corrosion. We then see in the potential–dimension diagram that pitting corrosion progresses in the region in which the corrosion potential is more positive than both the pit-repassivation potential ER and the critical depassivation potential EP∗ , whereas it repassivates back to the passive state in the region in which the corrosion potential stands more negative than the pit-repassivation potential ER and more positive than the critical depassivation potential EP∗ . In general, crevice corrosion breaks out in the region where the corrosion potential, Ecorr , is more positive than the crevice protection potential, Ecrev , at which the crevice solution is acidiﬁed to the passivation–depassivation pH of the crevice metal. We see in Figure 1.10 that no crevice corrosion is expected to break out in the region where the corrosion potential is more negative than the crevice protection potential. A corroding crevice may be made passive by shifting its corrosion potential into the region more negative than the crevice protection potential Ecrev . 1.5 Corrosion Rust 1.5.1 Rust in Corrosion Metallic corrosion in general produces metal ions oxidized in the hydrated form and then precipitates a mass of corrosion rust in the solid form. Hydrated metal ions are mostly hard Lewis acids and tend to combine with chemical species of hard Lewis bases such as hydroxide ions, chloride ions, sulfate ions, and phosphate ions to form somewhat covalent or ionic compounds in the soluble or insoluble state. Both soluble and insoluble corrosion products inﬂuence the subsequent progress in metallic corrosion, causing either corrosion acceleration or inhibition [38–40]. We examine in this chapter insoluble corrosion products, that is, corrosion rust. Localized corrosion normally involves the transport of hydrated ions in the corrosion cell: anions migrate from the cathodic reaction site to the anodic reaction site, and cations migrate in the reverse direction. In the presence of a substantial mass of corrosion rust on the metal surface, the ionic migration occurs through the rust precipitate, and the occluded solution directly in contact with the metal under the rust may change its concentration in aggressive ions if the ions migrate selectively across the rust. The ion-selective nature of the rust, therefore, plays an inﬂuential role in the corrosion of rust-covered metals. Corrosion rust in general is more or less ion selective, and its ion selectivity is determined by the ﬁxed ionic charge in the more-or-less porous rust. The rust is anion selective if the ﬁxed charge is positive, while it is cation selective if the ﬁxed 19 20 1 Basics of Corrosion Chemistry charge is negative. Aluminum oxide is anion selective in neutral sodium chloride solution and turns to be cation selective in basic sodium hydroxide solution . Oxides such as hydrous ferric oxide, nickel oxide, and chromic oxide are anion selective in neutral chloride solution [42–44]. The ion selectivity of corrosion rust is normally estimated in terms of the transference number, τ , of migrating ions through the rust. It is found with a hydrous ferric oxide layer that τCl− = −0.94 and τNa+ = 0.06, indicating that ferric oxide is anion selective in neutral sodium chloride solution . The transference number of water, τH2 O , also estimates the osmotic ﬂow of water through the rust . Normally, metal hydroxides are anion selective in acidic solution and turns to be cation selective beyond a certain pH, called the isoelectric point pHiso ; pHiso = 10.3 for ferric oxide, and pHiso = 5.8 for ferric–ferrous oxide . Because of its effect on the ionic ﬁxed charge, the adsorption of multivalent ions exerts a signiﬁcant role on the ion selectivity of hydrous metal oxides. We see, for instance, that hydrous ferric oxide that is anion selective in neutral chloride solution turns to be cation selective with the adsorption of multivalent anions such as divalent sulfate ions, divalent molybdate ions, and trivalent phosphate ions [44, 47]. Metallic corrosion, as mentioned earlier, requires not only ionic transfer and migration but also electronic transfer at the surface of metals and rust deposits. It appears that corrosion rust mostly falls in the category of electronic semiconductors, whose electronic energy band structure differs from that of metals. For metals, the Fermi level, εF , (the electrode potential, E,) is in the conduction band where electrons are freely mobile, whereas for semiconductors, the Fermi level, εF , is located in the forbidden band gap where no freely mobile electrons are allowed to be present. The cathodic reaction involving electron transfer, therefore, proceeds differently on the metal and on the semiconductor. Metallic corrosion receives, as a result, an inﬂuence from the electron-selective nature of the rust. It is also apparent that the electrode potential of the rust formed on the metal may be either more positive or more negative than the corrosion potential of the metal, depending on whether the rust is n-type or p-type. Normally, iron oxide and zinc oxide are n-type oxides, while nickel oxide and copper oxide are p-type oxides. The presence of semiconducting rust in contact with metals may have an electronic inﬂuence to a certain extent on the metallic corrosion. We will discuss in the following sections how the ionic and the electronic character of corrosion rust affect metallic corrosion. 1.5.2 Ion-Selective Rust Let us suppose that anodic metal corrosion is in progress under an anion-selective rust layer in aqueous solution containing chloride ions, with the cathodic reaction occurring somewhere away from the anodic corrosion site. The anodic metal dissolution current in the local corrosion cell carries chloride ions from the outside solution through the corrosion rust layer into an occluded solution under the layer, as schematically shown in Figure 1.11. Accumulation of chloride ions in the occluded solution under the rust layer ﬁnally reaches a stationary level at which 1.5 Corrosion Rust M Win M M2+ Rust Wout Cl Win M M2+ Rust − Wout Cl H2O − H2O H+ H+ Anion-selective rust (a) M Cation-selective rust (b) Figure 1.11 Anion-selective and cation-selective rust layers on corroding metals: (a) anion-selective rust makes the occluded water acidify and (b) cation-selective rust makes the occluded water basify; M is the metal, Win is the occluded water under the rust, and Wout is the water outside the rust. the inward migration equals the outward diffusion of the ions. Furthermore, the inward chloride-ionic current carries water molecules by an electro-osmotic ﬂow into the occluded solution. The ﬁnal steady concentration of chloride ions under the anion-selective rust layer is thus determined by the ratio of the transference number, τCl− , of chloride ions to the transport number, τH2 O , of water molecules for the layer . As the local chloride ion concentration increases under the anion-selective rust layer, the occluded solution acidiﬁes and eventually accelerates the corrosion of the underlying metal. In order to prevent metallic corrosion due to the enriched chloride ions from occurring under the anion-selective rust, we need to make the rust less anion selective or turn it cation selective by some means such as the adsorption of multivalent anions on the rust, as mentioned earlier. We next consider a precipitate of cation-selective rust that covers over the surface of corroding metal. The anodic ion transport carries no chloride ions inward through the rust layer, but mainly carries hydrated hydrogen ions (protons) migrating outward from the occluded solution into the outside solution. No accumulation of both chloride and hydrogen ions is thus expected to occur in the occluded solution, where the depression of hydrogen ions causes the basiﬁcation of the solution and stimulates rust precipitation. Furthermore, the electro-osmotic outward water ﬂow along with the hydrogen ion migration counteracts the inward water diffusion into the occluded solution. Dehydration of the occluded solution may thus occur, resulting in the depletion of water required for anodic metal dissolution, which may suppress the corrosion of the underlying metal. Metallic corrosion sometimes produces a bipolar rust layer consisting of an anion-selective inner layer and a cation-selective outer layer. The bipolar rust layer may be realized by means of the adsorption of multivalent anions, which turns an outer rust layer cation selective on the inner anion-selective rust layer. The ionic bipolar layer, just like a p–n electronic junction that adjusts electronic 21 22 1 Basics of Corrosion Chemistry transport in semiconductors, rectiﬁes the ionic current across the bipolar junction, suppressing in the anodic direction the ionic migration across the rust layer . Furthermore, the high barrier for ionic transport generates at the bipolar junction a high electric ﬁeld and makes the bipolar layer dehydrate into a layer of compact corrosion-resistive rust. We thus assume that the bipolar ion-selective rust layer is likely to inhibit metallic corrosion, bringing the metal into the passive state. It is an observed fact that pitting corrosion in stainless steel containing molybdenum is inhibited by the molybdate ion adsorption that makes an outer rust layer cation selective on the original, anion selective rust deposit [49, 50]. It is worth noting at the end that the ion-selective nature of corrosion rust remains valid as long as the concentration of migrating ions is comparable with or less than that of the ﬁxed charge in the rust. If the rust is so coarsely porous that the migrating ion may receive little inﬂuence from the ﬁxed charge, no ion-selective migration is expected to occur. In contrast, if the rust is so dense that no hydrated ions may penetrate into it, the normal solid-state diffusion of dehydrated ions will take over only under an extremely intense electric ﬁeld. 1.5.3 Electron-Selective Rust We suppose that metallic corrosion produces n-type semiconductor rust of metal oxides or hydroxides on the metal surface. The corrosion potential, Ecorr , of an isolated metal is usually different from the electrode potential of an isolated semiconducting oxide of the metal. Semiconductor oxide in general sets its electrode potential at around its ﬂat band potential, Efb , where no space charge arises in the semiconductor. For most metals and their oxides in practical use, the ﬂat-band potential of n-type oxides is more negative (cathodic) than the corrosion potential of the metals. The n-type rust oxide in contact with the metal consequently shifts the corrosion potential more negative to equate the Fermi level, εF , of the metal with that of the semiconductor oxide, thus giving rise to a space charge layer in the semiconductor oxide, as schematically shown in Figure 1.12. As a result of shifting the corrosion potential in the more negative direction, the n-type semiconductor rust appears to reduce the metallic corrosion, whose rate normally increases with the more positive potential. Furthermore, under the sunlight that injects photo-exited mobile holes (electron vacancies) in the valence band of electron energy levels in the semiconductor, the potential of the space charge layer is reduced in the semiconductor and the corrosion potential consequently shifts further in the more negative direction, resulting in a further decrease in the corrosion rate. Metallic corrosion in the active state usually increases as the corrosion potential shifts in the positive (anodic) direction, and in the passive state also, pitting corrosion occurs at more positive potentials than the pit-initiation potential, Epit . It is then advantageous for protecting metals from general and localized corrosion that the corrosion potential is made more negative by placing a mass of n-type semiconductor rust on the metal surface. It is also worth noting that for some n-type semiconductor oxides under photo-excitation, anodic water oxidation may 1.5 Corrosion Rust MO eC eF H2O esC ∆eF w eV MO M H2O esC eC eF eF eVs eC eF H2O esC M e eI eF eOX hν eVs eV (a) MO M (b) F pe* eV h (c) Figure 1.12 Electron energy diagrams for metal and n-type oxide in contact with each other in aqueous solution: (a) prior to contact; (b) posterior to contact; and (c) under photo-excitation; M is the metal, MO is the metal oxide, εF is the Fermi level, εF∗ is the quasi-Fermi level for photo-excited holes in oxide, εC is the conduction band edge level, εV is the valence band edge level, and εOX is the Fermi level of oxygen electrode reaction. occur producing gaseous oxygen even at potentials much more negative (cathodic) than the oxygen equilibrium potential. The anodic photo-excited water oxidation on the semiconductor, if coupled with cathodic oxidant reduction on the metal, may take over the anodic metal dissolution, and hence the metal may be protected from corrosion. We see that metallic copper and stainless steel were prevented from corrosion when they were brought into contact with n-type titanium oxide [50, 51]. The effectiveness of corrosion protection due to the n-type semiconductor, by its nature, depends on the ratio of the surface area of the metal to the semiconductor oxide. For stainless steel in contact with an n-type semiconductor of titanium oxide, effective corrosion inhibition was observed at the metal–oxide area ratio less than one tenth . For most metal oxides and hydroxides of p-type semiconductors, in contrast, the ﬂat band potential, Efb , is more positive (anodic) than the corrosion potential, Ecorr , of the metals. The corroding metal hence shifts its corrosion potential in the more positive (anodic) direction when it is brought in contact with a mass of p-type semiconductor oxide. Photo-excitation, in addition, further shifts the corrosion potential in the more positive direction. Metallic corrosion may then be accelerated if some p-type semiconductor rust is formed on the metal surface. In particular, pitting corrosion that occurs beyond the pit-initiation potential may break out in the presence of p-type semiconductor oxides on the metal. We also note that the photo-excitation of electrons from the valence band into the conduction band of p-type semiconductor oxide makes it thermodynamically possible for the cathodic hydrogen ion reduction to occur on the photo-excited p-type oxide even in the potential range much more positive (anodic) than the equilibrium hydrogen potential. It appears, as a result, that metallic copper, which suffers no corrosion without oxygen gas, may corrode even in the absence of gaseous oxygen, with the cathodic hydrogen ion reduction occurring on a mass of p-type copper oxides in contact with the metal under sunlight or radioactive rays. Hydrogen ion reduction involves radioexcited electrons in the conduction band of the p-type copper oxide. 23 24 1 Basics of Corrosion Chemistry 1.5.4 Redox Rust Corrosion rust is occasionally subject to redox reactions on metals. We consider iron rust consisting of hydrous ferrous and ferric oxides, which are sensitive to reduction–oxidation reaction on the corroding iron surface. − Fe(OH)3 + H+ aq + eM = Fe(OH)2 + H2 O (1.26) For the redox reaction to occur, electrons and hydrogen ions will have to migrate through the hydrous oxide toward the reaction partners. In the cathodic reaction, hydrogen ions and electrons both migrate to ferric hydroxide to form ferrous hydroxide releasing water. The anodic reaction, inversely, draws both hydrogen ions and electrons out of ferrous hydroxide, with hydrogen ions migrating outward to the aqueous solution and electrons migrating inward to the metal surface. The reaction rate may thus be controlled by either hydrogen ion migration or electronic conduction in the redox rust. The electrode potential of the ferric–ferrous redox reaction is normally more positive than the corrosion potential of metallic iron. The redox oxide in contact with the metal hence makes the corrosion potential of the metal more positive, and it also provides the metal corrosion with the cathodic reaction as follows: − Fe → Fe2+ aq + 2eM anodic reaction − 2Fe(OH)3 + 2H+ aq + 2eM → 2Fe(OH)2 + 2H2 O (1.27) cathodic reaction (1.28) The ferrous oxide thus reduced may then be oxidized by atmospheric gaseous oxygen to form ferric oxide on the metal. − anodic reaction (1.29) 2Fe(OH)2 + 2H2 O → 2Fe(OH)3 + 2H+ aq + 2eM 1 − O2 + 2 H+ (1.30) aq + 2eM → H2 O cathodic reaction 2 The rate of the cathodic reduction of hydrous ferric oxide may be greater than the rate of the cathodic reduction of gaseous oxygen that normally occurs on the metal surface, hence the corrosion rate of metallic iron may be greater in the presence of ferric–ferrous redox oxide than in its absence on the metal surface. It is received understanding that the presence of redox rust may accelerate the corrosion of metals. 1.6 Atmospheric Corrosion 1.6.1 Atmospheric Corrosion Chemistry Metallic iron and steel corrode in the moist atmosphere. The corrosion initially produces hydrated ferrous ions at the anode part and hydrated hydroxide ions at 1.6 Atmospheric Corrosion the cathode part where air–oxygen is reduced to hydroxide ions, OH− aq . Hydrated + ferrous ions in general arise in a variety of forms, such as Fe2+ aq , Fe(OH)aq , − 0 Fe(OH)2,aq , and Fe(OH)3,aq , depending on the pH of the solution. As the ferrous ion concentration exceeds its solubility limit, gel-like ferrous hydroxide, Fe(OH)2,gel , precipitates out on the metal surface. According to thermodynamic calculations, gel-like ferrous hydroxide in pure water remains in equilibrium at pH 9.31 with its solubility at 1.27 × 10−5 mol dm−3 . The hydrated ferrous ions initially formed in corrosion then air-oxidize into the solid precipitate of ferric hydroxide, Fe(OH)3,solid . − + 2OH (1.31) 4 Fe2+ aq aq + O2 + 2H2 O → 4Fe(OH)3,solid − The term Fe2+ + 2OH aq denotes the initial corrosion products at both anode aq and cathode parts. In the presence of a fair amount of gel-like ferrous hydroxide, Fe(OH)2,gel , which maintains the solution at pH 9.31, the corrosion-produced ferrous ions in the hydrated form readily air-oxidize into the solid precipitate of ferric hydroxide, Fe(OH)3,solid , and simultaneously, the pH of the solution changes to 7 with the solubility limit of ferric hydroxide at 1.20 × 10−8 mol dm−3 . The ferric hydroxide precipitate thus formed gradually dehydrates into a mass of ferric oxyhydroxide. Fe(OH)3,solid → FeOOHsolid + H2 O (1.32) Solid ferric oxyhydroxide FeOOHsolid occurs in a variety of compounds such as α-FeOOH, β-FeOOH, γ -FeOOH, and amorphous FeOOH. A mass of α-FeOOH is the most stable, β-FeOOH is formed in the presence of chloride ions, γ -FeOOH is relatively stable, and an aggregate of amorphous FeOOH consists of extremely ﬁne α-FeOOH particles. The ferric oxyhydroxide thus formed in the early stage of corrosion tends to aggregate into a mass of dense solid precipitate in the pH range of 7–9.31, in which the oxyhydroxide retains almost no surface charge on it and hence readily coagulates into a mass of its precipitate . The solubility limit of α-FeOOH is 1.51 × 10−13 mol dm−3 and is much smaller than that of ferric hydroxide Fe(OH)3,solid . Furthermore, the gel-like ferrous hydroxide of Fe(OH)2,gel formed in an early stage of corrosion air-oxidizes and dehydrates into magnetite, Fe3 O4,solid , whose solubility limit is 1.10 × 10−13 mol dm−3 at pH 9.31 . 6Fe(OH)2,gel + O2 → 2Fe3 O4,solid + 6 H2 O (1.33) The magnetite thus formed may be more or less electrochemically reactive, absorbing and desorbing hydrogen ions and electrons as well. For metallic iron and steel containing alloying transition metal, M, atmospheric corrosion oxidizes the alloying metal into ferrite, MFe2 O4 , which then takes part in the rusting process. The ferrite may come out not only from the alloying elements but also from surface-coating substances on the metal. 2 M(OH)2,solid + 4Fe(OH)2,solid + O2 → 2MFe2 O4,solid + 4 H2 O (1.34) 25 26 1 Basics of Corrosion Chemistry The solubility of transition metal ferrites, such as ZnFe2 O4 , is as small as that of α-FeOOH . We see that, although occupying a minor concentration, transition metal ferrites play a signiﬁcant role in developing anticorrosion rust in weathering steels as mentioned in the following sections . Atmospheric corrosion normally proceeds in the cycles of wet and dry environments. According to what is called the Evans model , the anodic metal dissolution in the wet period is coupled with the cathodic reduction of ferric oxyhydroxide into reactive magnetite. − Fe → Fe2+ aq + 2eM 8FeOOH + Fe2+ aq + anodic reaction 2e− M → 3Fe3 O4 + 4H2 O (1.35) cathodic reduction (1.36) In the dry stage, the reactive magnetite air-oxidizes into ferric oxyhydroxide. − 4Fe3 O4 + 8H2 O → 12FeOOH + 4H+ aq + 4eM O2 + 2H2 O + 4H+ aq + 4e− M anodic oxidation → 4 H2 O cathodic reaction (1.37) (1.38) Combining the wet process with the dry process, we obtain the overall wet–dry corrosion process. 4Fe + 3O2 + 2H2 O → 4FeOOH (1.39) It is mainly iron oxyhydroxide rust that occurs in the atmospheric corrosion of metallic iron and steel. In general, atmospheric corrosion frequently develops the rust into a multilayered structure composed of a variety of iron oxides, hydroxides, and oxyhydroxides mentioned above. It is also observed that as the rusting progresses the corrosive hydroxide rust gradually turns into the more corrosion-resistive rust consisting mainly of α-FeOOH and amorphous FeOOH. The aged rust grows in an imbricate pattern, and the received wisdom is that the smaller imbricate scale provides weathering steels with more corrosion-resistive character. 1.6.2 Weathering Steel Corrosion Air pollutants such as chloride and sulfate, if present in the atmospheric moisture, penetrate the rust layer and create an anode channel for local corrosion. As the anodic metal dissolution progresses, the chloride and sulfate ions tend to accumulate in the anode channel where the aqueous solution acidiﬁes. The concentrated ferrous chloride ions at 1 mol dm−3 solution acidiﬁes the solution at pH 4.75, where no ferrous hydroxide is allowed to precipitate in the solid state because of − its solubility greater than 1 mol dm−3 . Hydrated ferrous chloride, Fe2+ aq + 2Claq , dissolved in local corrosion then gradually air-oxidizes and precipitates into ferric hydroxide rust in the anode channel, simultaneously producing hydrochloric acid − H+ + Cl aq . aq − − + (1.40) 4 Fe2+ aq + 2Claq + O2 + 10H2 O → 4Fe(OH)3,solid + 8 Haq + Claq 1.6 Atmospheric Corrosion The acidiﬁed anode channel itself, however, still maintains a signiﬁcant concentration of hydrated ferrous and ferric ions. These hydrated ions gradually leak out of the anode channel and air-oxidize into corrosion rust outside the anode channel. A model calculation estimates for the total concentration of corroded iron at 1 mol dm−3 that air-oxidation ﬁnally gives rise to the solution that contains −3 of FeOH+2 0.590 mol dm−3 of Fe+3 aq and 0.096 mol dm aq at the acidic level of pH 1.41 . In the calculation, one-third of the corroded iron precipitates as gel-like ferric hydroxide, Fe(OH)3,solid , in the anode channel at pH 1.41. Owing to its substantial surface charge in acidic solution, the gel-like ferric oxide assumes almost no aggregation into solid precipitates but disperses itself in the acidiﬁed anode channel, gradually dehydrating into β-FeOOH. The gel-like β-FeOOH then diffuses out forming a ﬂowing mass of nonprotective yellow rust on the metal surface. The remaining two thirds of corroded iron remains in the form of soluble complexes of ferric ions and diffuses out of the anode channel to precipitate into several varieties of fresh corrosion rust in the neutral solution outside the aged rust layer. In the anode channel containing acidiﬁed chloride ions and ferric ions, metallic iron corrodes with the cathodic oxidant reduction of hydrogen ions and ferric ions. − − 2+ (1.41) Fe + 2 H+ aq + 2Claq → Feaq + 2Claq + H2 − − 2+ Fe + 2Fe3+ aq + 6Claq → 3Feaq + 6Claq (1.42) The acidic corrosion reactions continue occurring as long as the anode channel keeps its solution sufﬁciently acidic. Weathering steels are normally subject to cyclic wet–dry corrosion in the atmosphere. In the wet period, they corrode locally, producing yellow rust that ﬂows out of the aged rust layers on the steels. In the dry period, on the other hand, the freshly formed rust dehydrates and air-oxidizes into a dense rust layer. The corrosion rust develops, as a result, into a multilayered structure successively consisting of dense and coarse rust layers formed in the dry and wet periods. Long-term observations of atmospheric corrosion of steels show that a linear bilogarithmic relation holds between the corrosion weight loss or penetration, wcorr , and the time, t, of corrosion for 20–30 years [56, 57]. wcorr = k1 tk2 log wcorr = A + B log t (1.43) Parameters k1 , k2 , A, and B are dependent on the type of steel materials and on the corrosion environments. No theoretical background has so far been made clear of Eq. (1.36), which, however, can be used to predict atmospheric corrosion for longer periods. 27 28 1 Basics of Corrosion Chemistry 1.6.3 Anticorrosion Rust It comes out of the foregoing discussion that the key point for weathering steel corrosion is to make the soluble product of ferrous ions air-oxidize as soon as possible into insoluble ferric hydroxide, which eventually turns to be anticorrosion rust on the metal surface. In general, the rate of air-oxidation of hydrated ferrous ions is much greater in neutral solution than in acid solution where no air oxidation of the ions virtually occurs. Once gel-like ferric hydroxide and ferrous hydroxide are formed in water, the solution remains around pH 7–9.31 where the air oxidation rate of ferrous ions is great. In the presence of chloride ions, however, the solution acidiﬁes in the anode channel and hence reduces the rate of the air-oxidation of ferrous ions, eventually counteracting the formation of anticorrosion rust. It is found that the presence of cupric ions, Cu2+ , and phosphate ions, PO3− 4 , catalytically accelerates the air-oxidation of ferrous ions even in acid solution . Weathering steels usually contain copper and phosphorus as alloying elements, which dissolve in the form of hydrated ions. The dissolved cupric and phosphate ions increase the rate of the air oxidation of ferrous ions into solid ferric hydroxide in the acidiﬁed anode channel, and they thus contribute to the formation of anticorrosion rust. For some reason not yet made clear, cupric ions Cu2+ also inﬂuence the coagulation of hydroxide and prevent ferric hydroxide from crystallizing into coarse nonresistive aggregates [59, 60]. The rust then remains amorphous and grows into a dense, void-free barrier layer of anticorrosive rust. In general, transition metal 2+ 3+ 2+ ions such as Ti4+ aq , Coaq , Craq , and Niaq , which all come from alloying elements in weathering steels, are also found to catalyze the formation of amorphous iron rust [61, 62]. It is the received understanding that the amorphous rust of ferric oxyhydroxide is much more anticorrosive than the coarse crystalline oxide rust. The ion-selective character of rust may also affect the corrosion of weathering steels. As mentioned earlier, the rust layer of cation-selective character prevents the occluded solution in the anode channel from being acidiﬁed and thus contributes to the formation of corrosion-resistive rust. The rust layer of anion-selective character, on the other hand, tends to make the anode channel acidify, thus retarding the formation of anticorrosion rust. It is, as mentioned earlier, the ﬁxed charge on the inner surface of the rust that generates the ion-selective nature of the rust. The ﬁxed charge depends on various factors such as adsorbed acid–base hydroxyl groups, nonstoichiometric surface composition, and speciﬁc adsorption of multivalent ions. In general, the surface charge of iron oxides and hydroxides is positive in the acidic range of water and negative in the basic range of water. The border pH, called the isoelectric point pHiso , differs with different sorts of iron rust. It appears that the more acidic is the isoelectric point the more corrosion resistive is the rust. It is noted that the speciﬁc adsorption of multivalent anions such as PO3− 4 and CrO2− , which come from alloying elements P and Cr in weathering steels, makes 4,aq the isoelectric point pH, pHiso , of the iron rust more acidic and hence contributes to the formation of anticorrosive rust layers on the steels. References 1.7 Concluding Remarks Corrosion science has made clear that metallic corrosion is in essence an electrochemical process combined with Lewis acid–base reactions at the interface between the metal and the environment, hence the corrosion potential plays a primary role in the process of corrosion. We have, however, a number of crucial issues to be studied to understand further the electrochemical and Lewis acid–base character of metallic corrosion at the molecular level. In this chapter we have discussed metallic corrosion only under normal conditions. We note that corrosion also occurs under mechanical stresses leading to environmental cracking, stress corrosion cracking, erosion corrosion, and cavitation corrosion. Furthermore, materials other than metals, such as semiconductors, ionic solids, ceramics, and organic polymers, are also more or less all subject to corrosion . References 1. Evans, U.R. (1937) Metallic Corrosion and 2. 3. 4. 5. 6. 7. 8. 9. Protection, Edward Arnold, London. Wagner, C. and Traud, W. (1938) Über die Deutung von Korrosionsvorgängen durch Überlagerung von elektrochemischen Teilvorgängen und über die Potentialbildung an Mischelektroden. Z. Elektrochem., 44 (7), 391–402. Wagner, C. (1974) Corrosion in aqueous solution and corrosion in gases at elevated temperature–analogies and disparities. Werkst. Korros., 25 (3), 161–165. Pourbaix, M. (1966) Atlas of Electrochemical Equilibria in Aqueous Solutions, Pergamon Press, Oxford. Garreles, R.M. and Christ, C.L. (1965) Solutions, Minerals and Equilibria, Harper & Row, London, p. 172. Kaesche, H. (1979) Die Korrosion der Metalle, 2 Auﬂage, Spring-Verlag, New York, p. 122. Sato, N. (1989) Toward a more fundamental understanding of corrosion processes. Corrosion, 45, 354–368. Jensen, W.B. (1980) The Lewis Acid-Base Concepts, John Wiley & Sons, Inc., New York, pp. 112–336. Okamoto, G., Shibata, T., and Sato, N. (1969) Reports of Asahi Glass Foundation for Industrial Technology, vol. 15, 10. 11. 12. 13. 14. 15. 16. Asahi Glass Foundation for Industrial Technology, Tokyo, pp. 207–230. Keir, J. (1790) Philos . Trans., 80, 259. Sato, N. and Okamoto, G. (1981) Electrochemical passivation of Metals, in Comprehensive Treatise of Electrochemistry, vol. 4 (eds J.O’M.B. Bockris and R.E. White), Plenum Publishing Corporation, New York, London, pp. 193–245. Sato, N. (1990) An Overview on the Passivity of Metals, in Passivity of Metals Part I, Corrosion Science, Vol. 31 (supplement) (eds N. Sato and K. Hashimoto), Pergamon Press, pp. 1–19. Sato, N. (1976) Passivity of Iron, Nickel, and Cobalt – General Theory of Passivity, in Passivity and its Breakdown on Iron and Iron Base Alloys (eds R. Staehle and H. Okada), NACE, Houston, pp. 1–9. Sato, N. (1982) Anodic breakdown of passive ﬁlms on metals. J. Electrochem. Soc., 129 (2), 255–260. Sato, N. (2001) The stability and breakdown of passive oxide ﬁlms on metals. J. Indian Chem. Soc., 78, 19–26. Okamoto, G. and Sato, N. (1959) Self-passivation of nickel in aerated aqueous solution. J. Jpn. Inst. Met., 23 (12), 725–728. 29 30 1 Basics of Corrosion Chemistry 17. Takahashi, H., Fujimoto, F., Konno, H., 18. 19. 20. 21. 22. 23. 24. 25. 26. 27. 28. and Nagayama, M. (1984) Distribution of aions and protons in oxide ﬁlms formed anodically on aluminum in a phosphate solution. J. Electrochem. Soc., 131 (8), 1856–1861. Ohtsuka, T., Masuda, M., and Sato, N. (1985) Ellipsometric study of anodic oxide ﬁlms on titanium in hydrochloric acid, sulfuric acid and phosphate solution. J. Electrochem. Soc., 132 (4), 787–792. Barr, T.L. (1979) An ESCA study of the termination of the passivation of elemental metals. J. Phys. Chem., 82 (16), 1801–1810. Fushimi, K. and Seo, M. (2001) Initiation of a local breakdown of passive ﬁlm on iron due to chloride ions generated by a liquid-phase ion-gun for local breakdown. J. Electrochem. Soc., 148 (11), B459–B456. Fushimi, K., Azumi, K., and Seo, M. (2000) Use of a liquid-phase ion-gun for local breakdown of the passive ﬁlm on iron. J. Electrochem. Soc., 147 (2), 552–557. Heusler, K.E. and Fisher, L. (1976) Kinetics of pit initiation at passive iron. Werkst. Korros., 27 (8), 551–556. Shibata, T. (1990) in Passivity of Metals Part I, Corrosion Science, Vol. 31 (supplement) (eds N. Sato and K. Hashimoto), pp. 413–423. Sato, N. (1976) Stochastic process of chloride-pit generation in passive stainless steel. J. Electrochem. Soc., 123 (8), 1197–1199. Hisamatsu, Y., Yoshii, T., and Matsumura, Y. (1974) in Localized Corrosion (eds R.W. Staehle, B.F. Brown, J. Kruger, and A. Agrawal), NACE, Houston, TX, pp. 420–436. Macdonald, D.D. (1992) The point defect model for the passive state. J. Electrochem. Soc., 139 (12), 3434–3449. Sato, N. (2001) Proceedings of the 2nd International Conference on Environment Sensitive Cracking and Corrosion Damage, Hiroshima, October 29–November 3, Japan Society Corrosion Engineering, pp. 49–54. Brennert, C. (1937) Method for testing the resistance of stainless steels to local 29. 30. 31. 32. 33. 34. 35. 36. 37. 38. corrosive attack. J. Iron Steel Inst., 135, 101–112. Hisamatsu, Y. (1976) in Passivity and its Breakdown on Iron and Iron Base Alloys (eds R.W. Staehle and H. Okada), NACE, Houston, TX, pp. 99–105. Engell, H.J. and Storica, N.D. (1959) Untersuchungen über Lochfrass an passiven Elektroden aus unlegiertem Stahl in chloridenhaltiger Schwefelsaure. Arch. Eisenhuttenwesen, 30 (4), 239–248. Sato, N. (1982) The stability of pitting dissolution of metals. J. Electrochem. Soc., 129 (2), 260–264. Laycock, H.J. and Newman, R.C. (1998) Temperature dependence of pitting potentals for austenitic stainless steels above their critical pitting temperature. Corrosion Sci., 40 (6), 887–902. Wallen, B. (2001) Critical Pitting Temperature of UNS S31600 in Different Sea Wateers, in Marine Corrosion of Stainless Steels, Pubication No. 33 (ed. D. Feron), European Federation of Corrosion, London, pp. 19–25. Tsujikawa, S., Sono, Y., and Hisamatsu, Y. (1987) in Corrosion Chemistry within Pits (ed. A. Turnbull), National Physical Laboratory, London, p. 171. Sato, N. (1995) The stability of localized corrosion. Corrosion Sci., 37 (12), 1947–1967. Sato, N. (2001) Potential-Dimension Diagram of Localized Corrosion, in Marine Corrosion of Stainless Steels, Publication No. 33 (ed. D. Feron), European Federation of Corrosion, London, pp. 185–201. Steinsmo, U., Rogno, T., and Drugli, J.M. (2001) Recommended Practice for Selection, Quality Control and Use of High-Alloy Stainless Steels in Sea Water Systems, in Marine Corrosion of Stainless Steels, Publication No. 33 (ed. D. Feron), European Federation of Corrosion, London, pp. 115–123. Sato, N. (2001) Ion-Selective Lust Layers and Passivation of Metals, in Passivity of Metals and Semiconductors, Proceedings 99-42 (eds B. Ives J.L. Luo, and J.R. Rodda), The Electrochemical Society, Inc., Pennington, pp. 281–287. References 39. Sato, N. (2002) Surface oxide ﬁlms af- 40. 41. 42. 43. 44. 45. 46. 47. 48. 49. 50. fecting metallic corrosion. Corrosion Sci. Technol., 31 (4), 262–274. Sato, N. (1987) Some concepts of corrosion fundamentals. Corrosion Sci., 27 (5), 354–368. Huber, K. (1955) Über anodisch erzeugte Silberbromidschichten. Ein Beitrag zur Frage nach der Struktur von Elektroden II, Art. Z. Elektrochem., 59 (7/8), 693–696. Suzuki, M., Masuko, N., and Hisamatsu, Y. (1971) Study on the rust layer on atmospheric corrosion resistant low alloy steels, part 4 behavior of electrolyte in rust. Boshoku Gijutsu (Jpn. Corrosion Eng.), 20 (7), 319–324. Yomura, Y., Sakashita, M., and Sato, N. (1979) Ion-selectivity in hydrated iron (II), (II-III), and (III) oxide precipitate membranes. Boshoku Gijutsu (Jpn. Corrosion Eng.), 28 (2), 64–71. Sakashita, M. and Sato, N. (1979) Ion-selectivity of precipitate ﬁlms affecting passivation and corrosion of metals. Corrosion, 35 (8), 351–355. Sakashita, M., Yomura, Y., and Sato, N. (1977) Ion-selectivity of hydrous iron (III) oxide precipitate membranes. Denki Kagaku (Jpn. Electrochem.), 45 (3), 165–170. Sakashita, M. and Sato, N. (1975) Water transference through nickel hydroxide precipitate membrane. J. Electroanal. Chem., 62 (1), 127–134. Sakashita, M. and Sato, N. (1977) The effect of molybdate anion on the ion-selectivity of hydrous ferric oxide ﬁlms in chloride solutions. Corrosion Sci., 17 (6), 473–486. Sakashita, M., Shimakura, S., and Sato, N. (1984) Proceedings 9th International Congress Metallic Corrosion, vol. 1, National Research Council of Canada, pp. 126–131. Clayton, C.R. and Lu, Y.C. (1989) A bipolar model of the passivity of stainless steels–III, the mechanism of MoO2− 4 formation and incorporation. Corrosion Sci., 29 (7), 881–898. Yuan, J. and Tsujikawa, S. (1995) Characterization of sol-gel-derived TiO2 51. 52. 53. 54. 55. 56. 57. 58. 59. 60. 61. 62. coatings and their photoeffectson copper substrates. J. Electrochem. Soc., 142 (10), 3444–3450. Fujisawa, R. and Tsujikawa, S. (1995) Mater. Sci. Forum, 183–189, 1076–1081. Tamura, H. (2008) The role of rusts in corrosion and corrosion protection of iron and steel. Corrosion Sci., 50, 1872–1882. Cornell, R.M. and Schwertmann, U. (1996) The Iron Oxides, Wiley-VCH Verlag GmbH, Weinheim, p. 224. Tamura, H. and Matijevic, E. (1982) Precipitation of cobalt ferrites. J. Colloid Interface Sci., 90 (1), 100–109. Evans, U.R. (1969) Mechanism of rusting. Corrosion Sci., 9 (12), 813–821. Fukushima, T., Sato, N., Hisamatsu, Y., Matsushima, T., and Aoyama, Y. (1982) Atmospheric Corrosion Testing in Japan, in Atmospheric Corrosion (ed. W.H. Ailor), A Wiley-Interscience Publication, John Wiley & Sons, Inc., New York, London, pp. 841–872. Pourbaix, M. (1982) in Atmospheric Corrosion (ed. W.H. Ailor), A Wiley-Interscience Publication, John Wiley & Sons, Inc., New York, London, pp. 107–121. Tamura, H., Goto, K., and Nagayama, M. (1976) Effect of anions on the oxygenation of ferrous ion in neutral solutions. J. Inorg. Nucl. Chem., 38 (1), 113–117. Furuichi, R., Sato, N., and Okamoto, G. (1969) Reactivity of hydrous ferric oxide containing metallic cations. Chimia, 23 (12), 455–465. Suzuki, I., Hisamatsu, Y., and Masuko, N. (1980) Nature of atmospheric rust on iron. J. Electrochem. Soc., 127 (10), 2210–2215. Ishikawa, T., Uemo, T., Yasukawa, A., Kandori, K., Nakayama, T., and Tsubota, T. (2003) Inﬂuence of metal ions on the structure of poorly crystallized iron oxide rusts. Corrosion Sci., 45, 1037–1045. Ishikawa, T., Maeda, A., Kandori, K., and Tahara, A. (2006) Characterization of rust on Fe-Cr, Fe-Ni, and Fe-Cu 31 32 1 Basics of Corrosion Chemistry bimary alloys by fourier transform infrared and N2 adsorption. Corrosion, 62, 559–567. 63. Sato, N. (2010) Fundamental Aspects of Corrosion of Metals and Semiconductors, in Electrocatalysis: Computational, Experimental, and Industrial Aspects, Surfactant Science Series, Vol. 149, Chapter 22 (ed. C.F. Zinola), CRC Press, Taylor & Francis Book, Inc., pp. 531–588.